expanded perlite/cork fillers applied to aerospace ... perlite/cork fillers applied to aerospace...
Click here to load reader
Post on 12-Jul-2020
Embed Size (px)
An Acad Bras Cienc (2018) 90 (3)
Anais da Academia Brasileira de Ciências (2018) 90(3): 3197-3206 (Annals of the Brazilian Academy of Sciences) Printed version ISSN 0001-3765 / Online version ISSN 1678-2690 http://dx.doi.org/10.1590/0001-3765201820170964 www.scielo.br/aabc | www.fb.com/aabcjournal
Expanded perlite/cork fillers applied to aerospace insulation materials
JULIANO R.A. PINTO1,2, NATALIA B. SANCHES3, MILTON F. DINIZ4, RÉGIS S. SANTOS2, JOSÉ I.S. DE OLIVEIRA1,2 and RITA DE CÁSSIA L. DUTRA1
1Departamento de Química, Instituto Tecnológico de Aeronáutica/ITA, Avenida Marechal do Ar Eduardo Gomes, 50, Vila das Acácias, 12228-900 São José dos Campos, SP, Brazil
2Divisão de Produção de Motores/APM, Estrada Municipal Lúcia Marcondes e Machado Penedo, s/n, Km 4,5, Varadouro, 12315-020 Jacareí, SP, Brazil
3Centro Universitário Sant’Anna/UNISANT’ANNA, Rua Voluntários da Pátria, 257, 02011-000 Santana, SP, Brazil 4Divisão de Química do Instituto de Aeronáutica e Espaço/IAE, Avenida Marechal do Ar
Eduardo Gomes, 50, Vila das Acácias, 12228-904 São José dos Campos, SP, Brazil
Manuscript received on November 26, 2017; accepted for publication on April 4, 2018
ABSTRACT Insulations for rocket motors such as Flexible Thermal Protections (FTPs) and Rigid Thermal Protection (RTPs) act as thermal barriers against the hyperthermal environment from the solid propellant combustion. FTPs present dual function: to extend RTPs performance, and to attenuate the propellant contraction. FTPs used in the Brazilian Space Program have asbestos in their composition since the 70´s; however, they are hazardous for human health. In this context, a mixture of Expanded Perlite (PExp) and Cork Powder (CP) was investigated as a replacement for asbestos. Results showed reduction about 21 % in density and an increase of 13 % in the ablative properties. The low mechanical properties not interfere in this type of FTP due to your function of attenuate the propellant contraction. Key words: asbestos replacement, cork, HTPB, insulation, perlite.
Correspondence to: Rita de Cássia Lazzarini Dutra E-mail: email@example.com
Thermal insulation of rocket motors main function is to act as a thermal barrier between the gases and the heat generated by the combustion of the solid propellant. It consists of several components to achieve this goal (Koo et al. 2010, Douglass 1976, Zhang et al. 2016).
The inside of the rocket motor, or booster, developed by a Brazilian Research Center (“Instituto de Aeronáutica e Espaço” - IAE) is
composed of an adhesive and thermal coating, called liner. The liner acts as an adhesive interface between the propellant and the Flexible Thermal Protections (FTPs) and Rigid Thermal Protection (RTPs) located in the front and rear domes. FTPs and RTPs are designed to protect the combustion chamber from high heat and mass flows (Palmerio 2017).
Composite materials have an extensive application in the aerospace industry as FTPs and RTPs because they combine good mechanical and thermal properties, besides being capable of forming a residual char layer during the pyrolysis
An Acad Bras Cienc (2018) 90 (3)
3198 JULIANO R.A. PINTO et al.
process. This char layer is mostly the responsible for the material ablative resistance (Silva et al. 2011, Yum et al. 2015, Natali et al. 2016a, Zhang et al. 2016).
Ablation is the process that delays the heat and mass transfer during the solid propellant combustion because of the slow and continuous consumption of the material that constitutes the thermal protection (Yum et al. 2015). This process is able to dissipate the high heat flux by the chemical and physical decomposition of the thermal insulation material, i.e., it transforms thermal energy in mass loss (Helber et al. 2012, Ahmad et al. 2014).
In addition to forming the char layer during the polymeric matrix pyrolysis, solid fillers added to the thermal insulation also act as a barrier to thermal insulation wear, mostly reducing the mechanical erosion process originated from the mass flow of the combustion gases (Yang et al. 2012, Borner et al. 2015).
Numerous materials have been tested and used in thermal insulation systems, such as glass, carbon and aramid fibers, silicon and iron oxides, carbides, asbestos, all with the purpose of acting as support for the char layer (Natali et al. 2016a, Deuri et al. 1988, Zhang et al. 2016).
In this context, cork is a biological material origin from the bark of the Quercus Suber L. tree. Used in insulation, its main function is to act as a protective layer. Because of its composition and chemical structure, cork is a versatile material in a wide range of applications, from bottle corks to thermal and acoustic insulation components (Pereira 2007, Sen et al. 2014).
From the chemical point of view, cork contains two categories of materials: the structural ones that confer stability and resistance to the cork cells, and the non-structural ones that confer other properties such as impermeability (Pereira 1992). Among the structural components, suberin and lignin are the most important on account of their stability during the pyrolysis and thermal degradation process of
the propellant combustion. They also are mostly responsible for the formation of the char layer (Silva et al. 2005, Mestre et al. 2006, Cordeiro et al. 1998, Sen et al. 2014).
For aerospace applications, cork stands as an interesting material, considering not only its characteristics of impermeability, low specific mass, thermal and acoustic insulation, but also its excellent ablative resistance, even when mixed with other components. However, it can reduce the mechanical properties of composites, which can be prevent using specific coupling agents. (Pereira 2007, Silva et al. 2011, Petit et al. 2007).
Perlite is another material with interesting properties. It is an amorphous mineral of volcanic origin rich in aluminosilicates and silicon oxide, and containing 2 to 5 % of water molecules trapped in its structure. Its name derives from the perlstein term and means rock with concentric cracks, similar to a broken pearl (Dogan and Alkan 2004, Arifuzzaman and Kim 2015a, Oktay et al. 2015, Celik et al. 2016, Maaloufa et al. 2015). When heated at temperatures above 870 °C, its structure becomes softer. The trapped water vaporizes expanding the beads of perlite about 10 to 30 times, thus, making it porous, hence forth known as expanded perlite (Gürsoy and Karaman 2016, Celik et al. 2016, Pilatos et al. 2016).
Expanded perlite is one of the few materials that associate the properties of lightness, sterility, thermal and acoustic insulation, resistance to fire, and the fact that it is incombustible. Thus, it is very important in fire resistant applications (Gürsoy and Karaman 2016, Shoukry et al. 2016).
Kallergis et al. (2013) and Sahraeian et al. (2013) verified that perlite tends to form a char layer on the pyrolyzed surface of a polyethylene composite, precisely because it exhibits good thermal resistance when subjected to the combustion and pyrolysis processes.
Although the results of Kallergis et al. (2013) and Sahraeian et al. (2013) concluded that perlite
An Acad Bras Cienc (2018) 90 (3)
PERLITE/CORK FILLERS APPLIED TO AEROSPACE INSULATION 3199
your composition 5 parts of expanded perlite and cork powder.
Quantities of expanded perlite and cork powder were determined based on the viscosity not superior to 45000 cP at 30 ºC for the casting of a full-size thermal protection.
The FTP reference is a material that has in your composition asbestos fiber and other fillers that give good mechanical and ablative properties, however, the asbestos in a carcinogenic material and these mix of fillers results in a FTP extremely dense and heavy, properties undesirable for aerospace applications.
Preparation of the Formulations: Initially, HTPB resin was heated and maintained around 60 °C, while fillers at 120 °C for 2 hours. HTPB resin, ferric acetyl acetonate catalyst Fe(C5H7O2)3 97 % (Aldrich), and the fillers were weighed and homogenized according to the formulations. They were then degassed for the addition and mixing of the TDI curing agent.
Specimens of each formulation were prepared for the mechanical tensile and elongation tests, as well as for the oxy acetylene torch ablation test. The specimens were cured at 60 °C for 24 hours, and then, were subjected to post cure at ambient conditions for another 7 days, so that the mechanical properties were fully achieved (Crespim et al. 2007).
produces a char layer during pyrolysis, they did not evaluate the use of perlite in thermal protection systems (TPS) applied to combustion chambers of rocket motors. Recently Natali et al. (2016a) published a review on the diverse types of ablative thermal protection systems for rocket motors, but the use of expanded perlite alone or mixed with any other material was not discussed.
In this scenario, the present study proposes the use of a cork powder and expanded perlite mixture for the development of flexible thermal protections for use in the interior of combustion chambers in solid propulsion rocket engines. The mixture provides dual purpose: tension relief between the solid propellant and the front and rear domes, and life extension of the rigid protection.
Furthermore, the formulation used is asbestos- free, which will allow the continuity of the Brazilian Space Program, given that asbestos has already bee